Artificial Neural Network Modeling for Predicting Wood Moisture Content in High Frequency Vacuum Drying Process - MDPI
Page content transcription
If your browser does not render page correctly, please read the page content below
Article Artificial Neural Network Modeling for Predicting Wood Moisture Content in High Frequency Vacuum Drying Process Haojie Chai 1 , Xianming Chen 2 , Yingchun Cai 1 and Jingyao Zhao 1, * 1 Ministry of Education, Key Laboratory of Bio-Based Material Science and Technology, College of Material Science and Engineering, Northeast Forestry University, Harbin 150040, China; email@example.com (H.C.); firstname.lastname@example.org (Y.C.) 2 College of Information and Computer Engineering, Northeast Forestry University, Harbin 150040, China; email@example.com * Correspondence: firstname.lastname@example.org; Tel./Fax: +86-451-8219-1002 Received: 5 December 2018; Accepted: 26 December 2018; Published: 29 December 2018 Abstract: The moisture content (MC) control is vital in the wood drying process. The study was based on BP (Back Propagation) neural network algorithm to predict the change of wood MC during the drying process of a high frequency vacuum. The data of real-time online measurement were used to construct the model, the drying time, position of measuring point, and internal temperature and pressure of wood as inputs of BP neural network model. The model structure was 4-6-1 and the decision coefficient R2 and Mean squared error (Mse) of the training sample were 0.974 and 0.07355, respectively, indicating that the neural network model had superb generalization ability. Compared with the experimental measurements, the predicted values conformed to the variation law and size of experimental values, and the error was about 2% and the MC prediction error of measurement points along thickness direction was within 2%. Hence, the BP neural network model could successfully simulate and predict the change of wood MC during the high frequency drying process. Keywords: neural network; high frequency drying; moisture content; wood 1. Introduction Wood MC (moisture content) is one of the crucial indicators in the drying process as it has a direct impact on the stability of wood drying quality, and a reasonable control of MC can help in meeting the various quality requirements of actual wood products . High frequency vacuum drying is a joint drying technology with a fast drying rate, low energy consumption, and low environmental pollution , and is in widespread use throughout the wood drying industry . However, due to the interference of high frequency electromagnetic fields, the traditional MC online monitoring device cannot be used normally, which makes the online prediction and effective detection of wood MC problematic . Therefore, the research on the prediction model of wood MC is of great significance in the high frequency drying process. The wood structure is complex and it is difficult to establish a precise mathematical model through mathematical mechanism. An accurate control of MC requires precise mathematical models. The high frequency vacuum drying of wood is a non-linear, complex drying process, which is difficult to accurately express, control, or implement by using general mathematical methods . The concept of BP (Back Propagation) neural network comes from the biological system of brain, which is composed of numerous neurons that are connected to each other through synapses that process information. The neural network has decent characteristics for predicting nonlinear complex systems [6,7], and the model reflects the intrinsic connection of experimental data after a finite Forests 2019, 10, 16; doi:10.3390/f10010016 www.mdpi.com/journal/forests
Forests 2019, 10, 16 2 of 10 number of iterative calculations. It is not only strong at processing nonlinearity, self-organizing adjustment, adaptive learning, and fault-tolerant anti-noise [8–10] but also can effectively deal with nonlinear and complex fuzzy processes. An effective network prediction model can be established without any assumption or theoretical relationship analysis, based on the historical data and powerful self-organization integration capabilities [11,12]. Artificial neural networks are increasingly being used for modeling in the field of wood science. For instance, in the field of wood drying, Avramidis (2006)  predicted the drying rate of wood based on neural network construction model; Zhang Dongyan (2008)  constructed a neural network model for predicting wood MC during conventional drying; İlhan Ceylan (2008)  used neural network models to study wood drying characteristics; Watanabe (2013, 2014) [16,17] employed artificial neural network model to predict the final moisture content of Sugi (Cryptomeria japonica) during drying and evaluate the drying stress on the wood surface. Ozsahin (2017)  utilized artificial neural networks to successfully predict the equilibrium moisture content and specific gravity of heat-treated wood. The artificial neural networks are widely used in the study of conventional drying characteristics, stress monitoring, and MC prediction of wood ; however, the use of neural networks to predict changes in the wood MC during high frequency drying has been rarely studied. Hence, in order to provide a predictive model for the control of wood MC during high frequency drying, based on the BP neural network algorithm and using the real-time online measurement data, drying time, location of measuring point, and internal temperature and pressure of wood as the input to neural network model, the changes in the wood MC can be predicted. Also, the feasibility and prediction accuracy of the model was analyzed. 2. Materials and Methods 2.1. On-Line Monitoring of Wood Internal Temperature and Pressure Some uniform and defect-free Mongolian pine (Pinus sylvestris var. mongholica Litv.) were selected. The 200 mm ends were removed at both ends of the test piece, and the specifications were 120 × 120 × 500 mm specimens after sawing and planning, and the initial moisture content was 50%. As shown in Figure 1, five temperature pressure measuring points were uniformly preset at the center of the sample in the thickness direction. Drilling holes on the side of specimen with a 4 mm drill bit to depth of 60 mm (seeing Figure 1 for specific locations). Each measuring point was embedded with one of the pressure and temperature fiber sensors, and the locations where the sensors were in contact with the surface of wood were coated with silica gel to ensure good sealing. The data was recorded online through the optical fiber sensors. As shown in Figure 2, 1 is drying tank of high frequency vacuum with the diameter of 650 mm and length of 1350 mm; 2 and 4 are upper and lower plates respectively; and 3 is test material. The high frequency generator oscillates at the frequency of 27.12 MHz and outputs the effective power of 1 kW, which is powered by the center of electrode plate length. During the drying process, the wood control temperature was set to 55 ◦ C, the ambient pressure was set to 8 kPa, and the control of high frequency output time was set to stop for 2 min after a continuous oscillation for 7 min. In the early stage of drying, wood was quickly taken out and weighed after every 4 h, the real-time MC of wood was calculated, and the pressure and temperature values of five measuring points before the sample was taken out were recorded. In the middle stage of drying, the data were recorded once every 8 h; while, in the later stage of drying, the data were recorded once every 12 h. The drying was carried out for 204 h until wood MC was dried to 11.56%. The experiment was stopped and a total of 135 data were recorded.
Forests 2019, 10, 16 3 of 10 Forests 2018, Forests 2018, 9, 9, xx FOR FOR PEER PEER REVIEW REVIEW 33 of of 99 Figure 1. Figure Figure 1. Diagram 1. Diagram Diagram of of the wood of the the wood tested wood tested sample tested sample and sample and location and location of location of the of the sensors. the sensors. (1 sensors. (1 is (1 is the upper is the the upper layer upper layer layer measuring point; measuring measuring point; 222is point; isthe is theupper the uppermiddle upper middlelayer middle layermeasuring layer measuringpoint; measuring point;3 33isis point; isthe the the core core core layer layer layer measuring measuring measuring point; point; point; 44 4 is is is the the lower lower middle middle layer layer measuring measuring point; point; and and 5 5 is is the the lower lower layer layer measuring measuring the lower middle layer measuring point; and 5 is the lower layer measuring point). point). point). Figure 2. Figure 2. Drying Drying tank tank of of high high frequency frequency vacuum. vacuum. 2.2. BP 2.2. BP 2.2. Neural BP Neural Network Neural Network Model Network Model Model The The BP The BP(Back BP (BackPropagation) (Back Propagation) Propagation) model model model is currently is currently is currentlythe the most studied the most most and widely studied studied used artificial and widely and widely neural used artificial used artificial network model neural network neural . network model It has model . a powerful . It It has nonlinear has aa powerful mapping powerful nonlinear ability nonlinear mapping and the mapping ability qualities ability and and the of human the qualities qualities ofintelligence of human human such as self-learning, intelligence such asadaptive, associative self-learning, memory, adaptive, and parallel associative information memory, intelligence such as self-learning, adaptive, associative memory, and parallel information andprocessing. parallel It can imitate information the human processing. It processing. brain It cannervous can imitate system imitate the to the human store, human brain retrieve, brain nervousand process nervous system the system to information to store, with store, retrieve, retrieve, andan excellent processfault and process the the tolerance, information and information with is extremely with anan excellent suitable excellent fault for modeling fault tolerance, tolerance, andand isand control is extremely of complex extremely suitable suitable for systems for modeling . modeling and The Python and control control of of language has complex systems complex a rich systems . and powerful . The The Python class Python language library. language has It is an has aa rich interpreted, rich and and powerful interactive, powerful class and class library. pure library. ItIt is object-oriented is an an interpreted, interpreted, scripting programming interactive, interactive, and pure and language that scripting pure object-oriented object-oriented combines the best designlanguage scripting programming programming principlesthat language andcombines that ideas of several combines the best the different best design design languages principles and principles andis and widely ideas ideas of used in different of several several various fields different of software languages languages and is and isdevelopment widely used widely usedand application in various in various fields fields programming. of software of software Therefore, development development thisand paper and built the BP application application neural network programming. programming. model using Therefore, Therefore, thisPython this paper language paper the programming. built the built BP neural BP neural network network model using model using Python Python language language programming. programming. 2.2.1. Determination of Neuron Number 2.2.1.The 2.2.1. Determination Determination neural network of Neuron of Neuron Number Number prediction model in this paper uses a three-layer feedforward network structure, which includes an input layer, a hidden layer, and an output layer . The hidden The neural The neural network network prediction prediction model model in in this this paper paper uses uses aa three-layer three-layer feedforward feedforward network network layer can be further divided into a single hidden layer and multiple hidden layer according to the structure, which structure, which includes includes an an input input layer, layer, aa hidden hidden layer, layer, and and an an output output layer layer . . The The hidden hidden layer layer layer number. The multiple hidden layer is composed of multiple single hidden layers. Compared can be can be further further divided divided into into aa single single hidden hidden layer layer and and multiple multiple hidden hidden layer layer according according to to the the layer layer with a single hidden layer, a multiple hidden layer has a stronger generalization ability and higher number. The multiple hidden layer is composed of multiple single hidden layers. Compared with aa number. The multiple hidden layer is composed of multiple single hidden layers. Compared with prediction accuracy, but the training time is longer. The selection of hidden layers should be considered single hidden single hidden layer, layer, aa multiple multiple hidden hidden layer layer has has aa stronger stronger generalization generalization ability ability and and higher higher comprehensively based on the network accuracy and training time. For a simple mapping relationship, prediction accuracy, prediction accuracy, but but the the training training time time isis longer. longer. The The selection selection of of hidden hidden layers layers should should be be in case the network accuracy meets the requirements, the single hidden layer can be selected to speed considered comprehensively considered comprehensively based based on on the the network network accuracy accuracy and and training training time.time. For For aa simple simple up the process. For a complex mapping relationship, the multiple hidden layer can be selected to mapping relationship, mapping relationship, in in case case the the network network accuracy accuracy meets meets thethe requirements, requirements, the the single single hidden hidden layer layer enhance the network prediction accuracy. Therefore, according to the research requirements, the study can be can be selected selected to to speed speed up up the the process. process. For For aa complex complex mapping mapping relationship, relationship, the the multiple multiple hidden hidden chose a single hidden layer. layer can layer can be be selected selected to to enhance enhance the the network network prediction prediction accuracy. accuracy. Therefore, Therefore, according according to to the the The number of hidden neurons also has a certain impact on the network . The neuron number research requirements, research requirements, the the study study chose chose aa single single hidden hidden layer. layer. in the hidden layer is directly related to the predictive power of network model. If the number is The number The number of of hidden hidden neurons neurons alsoalso has has aa certain certain impact impact onon the the network network .. The The neuron neuron too high, it will not only increase the network training time but also the network will not converge number in number in the the hidden hidden layerlayer isis directly directly related related toto the the predictive predictive power power of of network network model. model. If If the the to the target error, resulting in an over-fitting. If the number is too small, the model training will be number is number is too too high, high, itit will will not not only only increase increase the the network network training training time time but but also also thethe network network will will not not converge to converge to the the target target error, error, resulting resulting inin an an over-fitting. over-fitting. If If the the number number is is too too small, small, the the model model training will training will bebe insufficient insufficient andand would would notnot be be able able to to completely completely express express thethe relationship relationship between between
Forests 2019, 10, 16 4 of 10 insufficient and would not be able to completely express the relationship between the input variables and output parameters, thus affecting the predictive ability of the model. Therefore, the determination of neuron number in hidden layer is particularly critical . The optimal neurons number was determined via trial and error method . The neuron number in hidden layer was set to 4~10, and the learning error and epoch of different nodes were tested by network training. The optimal node was obtained by comparison analysis. 2.2.2. Data Normalization The data obtained during the experiment were randomly divided into two data sets: a training group and a test group. The 101 test data of the training group accounted for 75% of the total data, while 34 data of the test group accounted for 25% of the total data. Each input sample usually has different physical meanings and dimensions; hence, in order to make each input sample have an equally important position and also to prevent the adjustment of the weight into the flat area of error, the input sample needs to be normalized . In addition, as the neurons of the BP neural network adopt the Sigmoid transfer function and the output is between [0, 1], it is also necessary to normalize the output samples (Equation (1)). X − Xmin X0 = (1) Xmax − Xmin where X0 is the X normalization value; Xmax and Xmin are the maximum and minimum values of X, respectively. The neurons in each layer are only connected to the neurons in the adjacent layer and there is no connection between the neurons in each layer. Also, there is no feedback connection between the neurons in each layer. The input signal first propagates forward to the hidden node and then through the transformation function. The output information of the hidden node is propagated to the output node and the output result is given after processing. In general, the Sigmoid transfer function (Equation (2)) is used on all nodes of hidden layer. In the output layer, all nodes use the linear transfer function Pureline. 1 f = (2) 1 + e− x where f represents the neuron output value and x represents the neuron input value. 2.2.3. Model Performance Analysis In the model correlation test, the model was evaluated by using the determination coefficient R2 and Mse (Mean squared error) of the training sample . The determination coefficient R2 is defined as: 2 ∑in=1 (ti − pi ) R2 = . (3) ∑in=1 t2i ∑in=1 p2i The Mean square error (Mse) is calculated as : 1 n n n∑ Mse = ( t i − p i )2 (4) =1 where ti (i = 1, 2, . . . , n) is the predicted value of the ith sample, pi (i = 1, 2, . . . , n) is the true value of the ith sample, and n is the total number of all samples. The decision coefficient is in [0, 1], and the closer the value to 1, the better the model performance, and the closer to 0, the worse the model performance. The smaller the sample Mean square error, the better the prediction performance and the better the model performance. The learning efficiency is set to 0.01.
Forests 2019, 10, 16 5 of 10 3. Results Forests Forests2018, and 2018,9,9,xxFOR Discussion FORPEER PEERREVIEW REVIEW 55 ofof 99 3.1. Determination 3.1. of Neuron Number 3.1.Determination DeterminationofofNeuronNeuronNumber Number The The corresponding relationship between the neuron number of hidden layer and the training Thecorresponding correspondingrelationship relationshipbetween betweenthetheneuron neuronnumber numberof ofhidden hiddenlayer layerand andthe thetraining training error error and epoch of neural network is shown in Figure 3. When the node number of hidden layer is 6, errorand andepoch epochof ofneural neuralnetwork networkisisshown shownin inFigure Figure3.3.When Whenthethenode nodenumber numberof ofhidden hiddenlayerlayerisis6,6, thethe training error is the smallest at 0.07355, and the epoch is 17, the network training is faster. These thetraining trainingerror errorisisthe thesmallest smallestatat0.07355, 0.07355,and andthetheepoch epochisis17, 17,the thenetwork networktraining trainingisisfaster. faster.These These results results show that the neural network model has superb generalization ability at this time ; hence, resultsshow showthatthatthe theneural neuralnetwork networkmodel modelhas hassuperb superbgeneralization generalizationability abilityatatthis thistime time; ;hence, hence, thethe node number ofhiddenhidden layerisis determined determined to be 6. According totothe node number of hidden layer, thenode nodenumber numberof of hiddenlayer layer is determinedto tobe be6.6.According According tothe thenode nodenumber numberof ofhidden hidden the structure layer, of neural network is shown in Figure 4. layer,the thestructure structureof ofneural neuralnetwork networkisisshown shownin inFigure Figure4.4. Figure 3.3.Correspondence Figure Figure 3. Correspondence between Correspondence betweenthe between network thethe networkerror network errorand error the and and number thethe of ofhidden number number of layer hidden hidden neurons. layer layer neurons. neurons. Figure Figure 4.4.BP (Back BPBP(Back (BackPropagation) Propagation) neural Propagation)neural neural network network networkstructure structure diagram structurediagram diagram(X 1: drying time; X2: measuring (X(X 1: drying time; time;X2X: 2measuring Figure 4. 1 : drying : measuring point pointposition; position; point X position; 3: temperature; X4: pressure; Y1: MC (moisture content)). X3X: temperature; : X temperature;4:Xpressure; : Y1:Y pressure; MC : MC(moisture content)). (moisture content)). 3 4 1 3.2. 3.2. 3.2. Model Model Model Performance Performance Performance Analysis Analysis Analysis TheThe The training trainingregression training regression map regression map mapfor for the forthetheBPBP neural neural BP network network neural network isis shown is shown in in Figure shown in Figure 5.5. The 5. The linear Figure The linear regression linear regression regression equation between experimental and the predicted value is y = 0.948x+1.24 while the equation equation between between experimental experimental and the and predictedthe predicted value is y =value 0.948x is + y = 1.24 0.948x+1.24 while the while determinationthe coefficient R2coefficient determination determination coefficient RR22 isisresults is 0.974. These 0.974. These These results 0.974.indicate that the results indicate that that the experimental indicate and the experimental predicted values experimental and and predicted fit well. The predicted values values fit fitwell. BP neural The TheBP network well. BP neural model neuralhas network a goodmodel network has hasaagood performance model and performance good can explain 97% performance and andof can theexplain can 97% 97%of ofthe above experimental explain the above experimental values . values above experimental values . . TheThe The predicted predicted predicted fitted curve fitted fitted curvefor curve forthe for theneural the neuralnetwork neural networkisis network isshown shownin shown inFigure Figure6. 6.6.The The remaining Theremaining remaining25% 25% 25%ofofthe of the the samples samples samples areare are predicted predicted predictedandand and compared comparedcomparedwithwith the the experimental the experimental with values. experimental values. The The predicted The predicted values. values values are predicted are consistent values are consistent with the variation and size of the experimental values. Initially, consistent with the variation and size of the experimental values. Initially, the BP neural network the BP neural network model modelcan cansimulate simulateand andpredict predictthe thechange changeof ofwood woodMC MCduring duringhigh highfrequency frequencydrying. drying.
Forests 2019, 10, 16 6 of 10 with the variation and size of the experimental values. Initially, the BP neural network model can simulate Forests 2018,and Forests 2018, 9, predict 9, xx FOR FOR PEER PEERthe change of wood MC during high frequency drying. REVIEW REVIEW 66 of of 99 Figure 5. Figure 5. Training Training regression graph of regression graph of BP BP neural neural network. network. Figure 6. Figure 6. Prediction Prediction fitting fitting curve curve of of BP BP neural neural network. network. 3.3. Prediction 3.3. Prediction of of Moisture Moisture Content Content Change Change During the During thedrying dryingprocess process of of wood, the free wood, waterwater the free is primarily discharged is primarily along the discharged largethe along capillary large system capillary above system theabove fiber saturation point. Thepoint. the fiber saturation bound Thewater in cell bound waterwalliniscell mainly wall discharged along the is mainly discharged microcapillary along system below the microcapillary systemthebelow fiber saturation point. Thepoint. the fiber saturation bound water The bound is affected water isby the hydroxyl affected by the hydroxyl interaction force in the amorphous region of cell wall . In the early stage ofthere interaction force in the amorphous region of cell wall . In the early stage of drying, is a drying, short is there accelerated drying section. a short accelerated drying The energyThe section. of high energyfrequency of high radiation frequencyisradiation basically isused to raise basically the used temperature of wood, and the drying rate is gradually increased from zero. to raise the temperature of wood, and the drying rate is gradually increased from zero. The middle The middle stage of drying is constant-speed stage of drying is drying section. The constant-speed dryingenergy of high section. Thefrequency energy ofradiation is basically high frequency used toisevaporate radiation basically the moisture in wood. The MC decreases rapidly and exhibits constant-speed used to evaporate the moisture in wood. The MC decreases rapidly and exhibits constant-speed drying tendency. This stage basically completes the evaporation process of moisture in wood. drying tendency. This stage basically completes the evaporation process of moisture in wood. In the In the later stage of drying, there is lessofwater later stage in wood, drying, there isand lessthe evaporation water in wood,rateandofthemoisture and therate evaporation drying rate of wood of moisture and thegradually drying decrease . rate of wood gradually decrease . The experimental The experimentaldata datais is input inputintointo the trained model the trained for simulation model verification. for simulation Figure 7Figure verification. presents 7 the curve of predicted and experimental values with time. In the early stage presents the curve of predicted and experimental values with time. In the early stage of drying, the of drying, the predicted values arevalues predicted slightlyarelower thanlower slightly the experimental values; in values; than the experimental the middle stage in the of drying, middle stage of thedrying, predicted the values are slightly higher than the experimental values; and in the later predicted values are slightly higher than the experimental values; and in the later stage of stage of drying, the predicted drying, values the have a slight predicted valueswave havemotion, a slightbut overall wave the value motion, but is basically overall thethe same value is as the experimental basically the same values. as the experimental values. Figure 8 displays the predicted error curve for the neural network (error = experimental value − predicted value ). The overall error range is −4%~6% and most of the data is concentrated between −2%~2%, which can basically meet the requirements of prediction accuracy in wood drying.
Overall, the predicted data could basically reflect the change trend of MC during the high frequency drying process. The prediction error is about 2%, which proves the feasibility of BP neural network model in MC prediction. Moreover, if the external environmental parameters in the 7high Forests 2018, 9, x FOR PEER REVIEW of 9 frequency drying process and the relevant parameters of wood itself are known, the trained neural network2019,model 10, 16the can ForestsOverall, be used predicted datato could predict the MC basically change, reflect thereby trend the change eliminating of MC the complicated during the 7high of 10 experimental frequency drying detection process process. and savingerror The prediction timeisand cost2%, about . which proves the feasibility of BP neural network model in MC prediction. Moreover, if the external environmental parameters in the high frequency drying process and the relevant parameters of wood itself are known, the trained neural network model can be used to predict the MC change, thereby eliminating the complicated experimental detection process and saving time and cost . Figure 7. Simulation results of BP neural network. Figure 8 displays the predicted error curve for the neural network (error = experimental value − predicted value ). The overall error range is −4%~6% and most of the data is concentrated between −2%~2%, which can basically meet the requirements of prediction accuracy in wood drying. Figure 7. Simulation results of BP neural network. Figure 8. Prediction error of BP neural network. 3.4. Analysis of Stratified Moisture Content Prediction Error Figure 9 shows the MC prediction error of measurement points along thickness direction. In the early and later stage of drying, Figure 8. Prediction the error errorand is positive of BP theneural network. network. predicted values are slightly less than the experimental values. In the middle stage of drying, the error is negative and the predicted values are Overall, 3.4. Analysis slightly larger ofthe predicted Stratified than dataContent Moisture the experimental could basically Prediction values. Among reflect Error these, thethechange error intrend of MCstage the middle during the high of drying is frequency the largest, drying followed process. by the The prediction early and later errorofisdrying. stage about In 2%,thewhich early proves and the feasibility middle stage of of BP drying, Figure 9 shows the MC prediction error of measurement points along thickness direction. In the neuralthe along network thicknessmodel in MC prediction. Moreover, iftop thetoexternal bottom,environmental parameters in the early and later stage direction of drying,ofthe test material, error fromand is positive the predicted the error values areincreases firstly, slightly less thanthen the high frequency decreases, then drying process increases, and anddecreases. then the relevantTheparameters results show ofM-type wood itself trend are with known, no clearthelaw, trained experimental values. In the middle stage of drying, the error is negative and the predicted valuesandare neural the errornetwork of the modelsurface upper can be measurement used to predict the MC point is thechange, smallest.thereby In the eliminating later stage thedrying, of complicated along slightly larger than the experimental values. Among these, the error in the middle stage of drying is experimental the thickness detection direction process andmaterial, saving time andtop cost to. the largest, followed by of thethe test early and later stagefrom of drying. bottom, the error In the early and is firstlystage middle reduced, then of drying, increased, along the and then decreased, thickness direction while of test the error atfrom material, the upper top to intermediate bottom, the layer error is the smallest. increases firstly, then 3.4. Analysis of Stratified Moisture Content Prediction Error Due to the difference in material properties at different locations decreases, then increases, and then decreases. The results show M-type trend with no clear law, and of the wood and the degree of Figure electromagnetic 9 shows the error of the upper the radiation,MC prediction themeasurement surface error of prediction accuracy measurement point is the of each points along measurement smallest. thickness In the laterpoint direction. stage isof different. In drying, along the But early and overall, later the stage prediction of drying, error the of MC error of is positive each layer and is the less predicted than 2%, values are indicating the thickness direction of the test material, from top to bottom, the error is firstly reduced, then slightly that theless than predictionthe experimental increased, andvalues. In the middle then decreased, while stage the of drying, error at thethe errorintermediate upper is negative and theispredicted layer values are the smallest. slightly larger than the experimental values. Among these, the error in the Due to the difference in material properties at different locations of the wood and the degree middle stage of drying is the of largest, followed by the early and later stage of drying. In the early electromagnetic radiation, the prediction accuracy of each measurement point is different. But and middle stage of drying, along the thickness overall, direction oferror the prediction test material, of MC offrom eachtop to bottom, layer is less the thanerror 2%,increases indicating firstly, that then decreases, the prediction then increases, and then decreases. The results show M-type trend with no clear law, and the error of the upper surface measurement point is the smallest. In the later stage of drying, along the thickness
Forests 2019, 10, 16 8 of 10 Forests 2018, 9, x FOR PEER REVIEW 8 of 9 direction accuracy of of the test each material, from measurement topistogood point bottom, andthe error can is firstly meet reduced,for the demand then increased, stratified and then moisture decreased, while content prediction. the error at the upper intermediate layer is the smallest. Figure 9. Error Figure analysis 9. Error of stratified analysis moisture of stratified content moisture prediction. content prediction. Due to the difference in material properties at different locations of the wood and the degree of 4. Conclusions electromagnetic radiation, the prediction accuracy of each measurement point is different. But overall, The BP neural network was used to simulate the wood MC during the high frequency drying the prediction error of MC of each layer is less than 2%, indicating that the prediction accuracy of each process. The drying time, the location of measuring point, and the internal temperature and pressure measurement point is good and can meet the demand for stratified moisture content prediction. of the wood were taken as input variables, while the wood MC was the output variable, 101 test data of the training group accounted for 75% of the total data, while 34 data of the test group accounted 4. Conclusions for 25% of the total data. The results showed that when the number of hidden layer of neurons was six, the The BP neural neural network network trainingwas usedwas error to simulate the wood the smallest MCBP and the during neuralthenetworks high frequency drying had better process. The drying time, the location of measuring point, and the internal stability. The error between the predicted and the experimental values was about 2% and the temperature and pressure of the wood stratified werecontent moisture taken as input variables, prediction error waswhile the 2%, within wood MC was which the output the model couldvariable, 101 testthe well simulate data change trend of wood MC during the drying process. In general, although the performance of woodfor of the training group accounted for 75% of the total data, while 34 data of the test group accounted 25%greatly varies of the total data. and the The results complex showedhas relationship that when not beenthe number of completely hidden layer elucidated, of neuronsneural the proposed was six, the neural network model network training is reliable and haserror was predictive a good the smallest and the BP neural networks had better stability. power. The error between the predicted and the experimental values was about 2% and the stratified moisture content Author predictionH.C. Contributions: errorandwas within X.C. 2%, and conceived which the model designed could well the experiments; simulate J.Z. performedthethe change trend of experiments; wood H.C. MC analyzed and Y.C. during thethedrying data andprocess. In general, wrote the paper. although the performance of wood varies greatly and the complex relationship has not been completely elucidated, the proposed neural network model is Funding: The Fundamental Research Funds for the Central Universities (Grant No. 2572018BB08) and the reliable National and has Natural a good Science predictive Foundation power. of China (Grant No. 31670562), financially supported this research. Acknowledgments: The authors Author Contributions: thank H.C. and X.C.Zhiqiang Huang conceived for the technical and designed support inJ.Z. the experiments; theperformed computer the field. experiments; H.C. and Y.C. analyzed the data and wrote the paper. Conflicts of Interest: The authors declare no conflict of interest. Funding: The Fundamental Research Funds for the Central Universities (Grant No. 2572018BB08) and the National Natural Science Foundation of China (Grant No. 31670562), financially supported this research. References Acknowledgments: The authors thank Zhiqiang Huang for the technical support in the computer field. 1. Xie, J. Study on Larch Wood Drying Models by Artificial Neural Network. Master’s Thesis, Northeast Conflicts of Interest: The authors declare no conflict of interest. Forestry University, Harbin, China, 2013. 2. Chai, H.J. Development and Validation of Simulation Model for Temperature Field during High References Frequency Heating of Wood. Forests 2018, 9, 327. 3. 1. Kong, Xie,F.X. J. Study StudyononLarch Wood Drying Technique Models by Artificial of Radio-Frequency VacuumNeural DryingNetwork. Master’sJ. Thesis, for Oak Veneer. Northeast Northeast. For. Forestry Univ. University, 2018, 6, 46. Harbin, China, 2013. 4. 2. Li, Chai, H.J. Development X.J. Characteristics and Validation of Microwave VacuumofDrying Simulation Model of Wood andfor Temperature Mechanism Field during of Thermal HighTransfer; and Mass Frequency Heating of Wood. Forests 2018, 9, 327. [CrossRef] China Environmental Science Press: Beijing, China, 2009; p. 65, ISBN 9787802099890. 5. 3. Yu,Kong, H.M. F.X. StudyStudy on Technique on Drying of Radio-Frequency Mathematical Vacuum Drying Model of Hawthorn for Oak Veneer. Using Microwave J. Northeast. Coupled with HotFor.Air Univ. and2018, 6, 46. Drying Machine Design. Ph.D. Thesis, Jilin University, Changchun, China, 2015. 6. Zhou, P. MATLAB Neural Network Design and Application; Tsinghua University Press: Beijing, China, 2013; p. 153, ISBN 9787302313632.
Forests 2019, 10, 16 9 of 10 4. Li, X.J. Characteristics of Microwave Vacuum Drying of Wood and Mechanism of Thermal and Mass Transfer; China Environmental Science Press: Beijing, China, 2009; p. 65. ISBN 9787802099890. 5. Yu, H.M. Study on Drying Mathematical Model of Hawthorn Using Microwave Coupled with Hot Air and Drying Machine Design. Ph.D. Thesis, Jilin University, Changchun, China, 2015. 6. Zhou, P. MATLAB Neural Network Design and Application; Tsinghua University Press: Beijing, China, 2013; p. 153. ISBN 9787302313632. 7. Poonnoy, P.; Tansakul, A. Artificial Neural Network Modeling for Temperature and Moisture Content Prediction in Tomato Slices Undergoing Microwave-Vacuum Drying. J. Food Sci. 2007, 72, E042–E047. [CrossRef] [PubMed] 8. Sablani, S.S.; Kacimov, A. Non-iterative estimation of heat transfer coefficients using artificial neural network models. Int. J. Heat Mass Transf. 2005, 48, 665–679. [CrossRef] 9. Rai, P.; Majumdar, G.C. Prediction of the viscosity of clarified fruit juice using artificial neural network: A combined effect of concentration and temperature. J. Food Eng. 2005, 68, 527–533. [CrossRef] 10. Shyam, S.; Sablani, M. Using neural networks to predict thermal conductivity of food as a function of moisture content, temperature and apparent porosity. Food Res. Int. 2003, 36, 617–623. 11. Hagan, M.T. Neural Network Design; PWS Publishing Company: Boston, MA, USA, 1996. 12. Fu, Z. Artificial neural network modeling for predicting elastic strain of white birch disks during drying. Eur. J. Wood Wood Prod. 2017, 75, 949–955. [CrossRef] 13. Wu, H.W.; Stavros, A. Prediction of Timber Kiln Drying Rates by Neural Networks. Dry Technol. 2006, 24, 1541–1545. [CrossRef] 14. Zhang, D.Y. Neural network prediction model of wood moisture content for drying process. Sci. Silva Sin. 2008, 44, 94–98. 15. İlhan, C. Determination of Drying Characteristics of Timber by Using Artificial Neural Networks and Mathematical Models. Dry Technol. 2008, 26, 1469–1476. 16. Watanabe, K. Artificial neural network modeling for predicting final moisture content of individual Sugi (Cryptomeria japonica) samples during air-drying. J. Wood Sci. 2013, 59, 112–118. [CrossRef] 17. Watanabe, K. Application of Near-Infrared Spectroscopy for Evaluation of Drying Stress on Lumber Surface: A Comparison of Artificial Neural Networks and Partial Least Squares Regression. Dry Technol. 2014, 32, 590–596. [CrossRef] 18. Ozsahin, S. Prediction of equilibrium moisture content and specific gravity of heat treated wood by artificial neural networks. Eur. J. Wood Wood Prod. 2018, 76, 563–572. [CrossRef] 19. Aghbashlo, M. Application of Artificial Neural Networks (ANNs) in Drying Technology: A Comprehensive Review. Dry Technol. 2015, 33, 1397–1462. [CrossRef] 20. Zhang, Z.Y. Research on Load Forecasting Analysis of Wuhai Power Grid Based on Artificial Neural Network BP Algorithm. Master Thesis, University of Electronic Science and Technology of China, Sichuan, China, 2008. 21. Bi, W. Research and Design of a Wood Drying Control System Based on Artificial Neural Network. Master’s Thesis, Jilin University, Changchun, China, 2011. 22. MATLAB Chinese Forum. 30 Case Analysis of MATLAB Neural Network; Beijing University of Aeronautics and Astronautics Press: Beijing, China, 2010. 23. Liu, T.Y. Improvement Research and Application of BP Neural Network. Master’s Thesis, Northeast Agricultural University, Harbin, China, 2011. 24. Fu, Z.Y. Study on Dry Stress and Strain of Birch Tree in Conventional Drying Process. Ph.D. Thesis, Northeast Forestry University, Harbin, China, 2017. 25. Zhang, T. Prediction Model of Moisture Content of Ginger Hot Air Drying Based on BP Neural Network and SVM. Master’s Thesis, Inner Mongolia Agricultural University, Hohhot, China, 2014. 26. Xu, X. Nonlinear fitting calculation of wood thermal conductivity using neural networks. Zhejiang Univ. (Eng. Sci.) 2007, 41, 1201–1204. 27. Gao, J.M. Wood Drying, 1st ed.; Science Press: Beijing, China, 2008; p. 10. ISBN 9787030205179. 28. Allegretti, O. Nonsymmetrical drying tests—Experimental and numerical results for free and constrained spruce samples. Dry Technol. 2018, 36, 1554–1562. [CrossRef]
Forests 2019, 10, 16 10 of 10 29. Cai, Y.C. Wood High Frequency Vacuum Drying Mechanism; Northeast Forestry University Press: Harbin, China, 2007. 30. Wang, Y. Prediction of Wood Moisture Content Based on BP Neural Network Optimized by SAGA. Tech. Autom. Appl. 2013, 32, 4–6. © 2018 by the authors. Licensee MDPI, Basel, Switzerland. This article is an open access article distributed under the terms and conditions of the Creative Commons Attribution (CC BY) license (http://creativecommons.org/licenses/by/4.0/).
You can also read
Next slide ... Cancel